084707-5 **Simulation** **of** **crack** **propagation** **in** alum**in**a J. Chem. Phys. 136, 084707 (2012) FIG. 2. Surface relaxations for the new potential compared **with** **ab** **in**itio calculations. Red: oxygen. Blue: alum**in**um. (a) (0001)-surface, **ab** **in**ito, (b) (0001)- surface, MD, (c) (0110)-surface, **ab** **in**ito, and(d)(0110)-surface, MD. two s**in**gle crystal elementary cells **with** mirror symmetry. The mirror plane is a (0001) oriented oxygen layer. Based on the mirror tw**in**, one can obta**in** the rotation tw**in** by shift**in**g one **of** the s**in**gle crystal elementary cells **in** the [0110] direction. For details **of** the **in**terface structures, see Ref. 4. As can be seen from T**ab**le II, the**ab** **in**ito calculated **in**terface energies **of** the basal tw**in**s agree well **with** the results from Ref. 4.The MD simulations **with** the new potential underestimate both energy values. But, the potential is **ab**le to qualitatively reproduce the relation **of** the two **in**terface energies: The **in**terface Downloaded 29 Feb 2012 to 129.69.47.171. Redistribution subject to AIP license or copyright; see http://jcp.aip.org/**ab**out/rights_and_permissions

084707-6 Hocker et al. J. Chem. Phys. 136, 084707 (2012) Stress (GPa) 50 40 30 20 10 0 **ab**-**in**itio [0001] **ab**-**in**itio [¯2110] **ab**-**in**itio [0¯110] MD [0001] MD [¯2110] MD [0¯110] 2 4 6 8 10 12 14 Stra**in** (%) FIG. 3. Stresses **of** stra**in**ed configurations **with** [0001] (green), [2110] (red), and [0110] (blue) stra**in** directions aga**in**st the stress tensor component **in** direction **of** stra**in**. The curves obta**in**ed **with** the new potential are marked **with** squares, those from **ab** **in**itio calculations **with** circles. energy **of** the mirror tw**in** (E m tw**in** ) is **ab**out two by three times the one **of** the rotation tw**in** (E r tw**in** ); that is why, the latter one is energetically favor**ab**le. IV. CRACK PROPAGATION A. **Simulation** conditions To **in**vestigate **crack** **propagation** **in** mode I at constant energy release rate, we prepared configurations **with** dimensions (b x , b y , b z )**of**21× 3 × 13 nm 3 which conta**in** **ab**out 80 000 atoms. Lateral planes **of** these cuboids are the (0001), (0110), and (2110) crystallographic planes. An elliptical **in**itial **crack** **of** 5 nm length **in** x-direction is **in**serted on one side **of** the samples by mov**in**g atoms **in** z-direction. The open**in**g **of** the **crack** is calculated **with** the Griffith criterion: In front **of** the **crack** tip, the sample is l**in**early stra**in**ed until the elastic energy due to stra**in** is equal to the Griffith energy G 0 which is twice the surface energy **of** the **crack** plane. This criterion was fulfilled at **ab**out 4% stra**in**. These structures are then relaxed to obta**in** the displacement field **of** a st**ab**le **crack**. Periodic boundary conditions are applied **in** the direction along the **crack** front, whereas fixed displacement boundary conditions are applied **in** the other directions. Initial configurations for **crack** **propagation** simulations **with** different energy release rates are obta**in**ed by a l**in**ear scal**in**g **of** this displacement field. Dur**in**g the **crack** **propagation** simulations, the NVE (constant number **of** particles, volume, and energy) ensemble and a start**in**g temperature **of** 0 K are applied. A timestep **of** 1 fs is used for all simulations. B. Cracks **in** a {1120} plane Initial **crack**s were **in**serted **in** a (2110) plane **with** **crack** **propagation** directions [0001] or [0110]. In both cases, the **in**itial **crack** is stationary at energy release rates up to 1.5 G 0 . Higher energy release rates lead to **crack** **propagation** **in** the **in**itial (2110) plane. It is known that the discrete character **of** **in**teratomic bonds which reveals itself **in** the so-called lattice trapp**in**g effect 40 can retard **crack** **propagation** to energy release rates beyond the critical energy release rate determ**in**ed by the Griffith criterion. As can be seen from Fig. 4(a), yet at high energy release rates bond break**in**g between the two **crack** lips is not cont**in**uous. Cha**in**s **of** atoms bridg**in**g the **crack** lips stay **in**tact dur**in**g the simulation. Furthermore, consider**ab**le disorder is observed at the result**in**g **crack** surfaces. In [0110] **propagation** direction, these effects are slightly more pronounced than **in** [0001] **propagation** direction. It cannot be ruled out that these very strong bonds are caused by **in**accuracies **of** the force field. However, the observation **of** **in**tact bonds bridg**in**g the **crack** lips agree **with** previous simulations **of** alum**in**a, where it was stated that these atomic cha**in**s were observed **in** experiments as well. 13 Our results show that **crack**s are **ab**le to propagate **in** (2110) planes **in** both [0001] and [0110] directions. This is **in** accordance **with** experiments, 2 where it turned out that **crack**s occur **in** {1120} planes, although these are not the preferred fracture planes. C. Cracks **in** a {0001} plane The {0001} planes are the closest packed planes **of** α-Al 2 O 3 ; therefore, cleavage **of** these planes is improb**ab**le. Our simulations confirm that **crack**s do not propagate **in** the (0001) plane **in** which the **in**itial **crack** was **in**serted **with** **crack** **propagation** directions [2110] or [0110]. At energy release rates below 1.7 G 0 , a damaged region **in** front **of** the **crack** tip is generated **with** atomic disorder similar to the case **of** the (2110) plane. However, the **crack** tip does not move. More **in**terest**in**g is the (0001)[0110] oriented **in**itial **crack** at higher energy release rates: As can be seen from Fig. 4(b), the **crack** propagates **in** a {1012} cleavage plane. Due to the boundary conditions, the **crack** surfaces cannot separate completely, but a row **of** oxygen atoms stays **in** the **crack** path. In contrast to the **crack**s **in** a {1120} plane, there is no disorder along the **crack** surfaces. The observed **crack** **propagation** **in** a {1012} cleavage plane agrees well **with** electron microscopy **in**vestigations 2 which revealed that fracture surfaces **of** the {1012} cleavage planes are frequently observed **in** alum**in**a. D. Cracks **in** a {1010} plane Cracks **in**itially **in**serted **in** a (0110) plane **in** [2110] direction propagate **in** this orientation start**in**g at energy release rates **of** 2.2 G 0 . In the case **of** a [0001] **crack** **propagation** direction (Fig. 4(c)), the movement **of** the **crack** tip was observed at energy release rates **ab**ove 1.9 G 0 . Similar to the case **of** the (0001)[0110] orientation, the **crack** changes its **propagation** plane. As can be seen **in** Fig. 4(c), the **crack** moves partially **in** the **in**itial (0110) plane, but also partially **in** a {1012} cleavage plane. As **in** the case **of** **crack**s **in** {1120} planes, the **in**itially (0110)[2110] or (0110)[0001] oriented **crack**s generate disorder at the **crack** surfaces dur**in**g **crack** **propagation**; some atomic bonds stay **in**tact across the **crack** open**in**g. Downloaded 29 Feb 2012 to 129.69.47.171. Redistribution subject to AIP license or copyright; see http://jcp.aip.org/**ab**out/rights_and_permissions